Crystal Structure Determination I


 Amos Cooper
 2 years ago
 Views:
Transcription
1 Crystal Structure Determination I Dr. Falak Sher Pakistan Institute of Engineering and Applied Sciences National Workshop on Crystal Structure Determination using Powder XRD, organized by the Khwarzimic Science Society, August 2007 ( 09/10/2010
2 Crystal Structure Determination The determination of an unknown structure proceeds in three major steps: 1. The shape and size of the unit cell are deduced from the angular positions of the diffraction lines. 2. The number of atoms per unit cell is then computed from the shape and size of the unit cell, the chemical composition of the specimen, and its measured density. 3. Finally, the position of the atoms within the unit cell are deduced from the relative intensities of the diffraction lines. The third step is generally the most difficult and there are many structures which are known only incompletely, in the sense that this final step has not yet been made. Size and Shape of the Unit Cell This step is same as the indexing of power diffraction pattern. It involves: The accurate determination of peak positions. Determination of the unit cell parameters from the peak positions. Bragg s Law Interplanar dspacing Systematic Absences
3 Bragg's Law When xrays are scattered from a crystal lattice, peaks of scattered intensity are observed which correspond to the following conditions: 1. The angle of incidence = angle of scattering. 2. The pathlength difference is equal to an integer number of wavelengths. The condition for maximum intensity contained in Bragg's law above allow us to calculate details about the crystal structure, or if the crystal structure is known, to determine the wavelength of the xrays incident upon the crystal.
4 Bravais lattices Crystals possess a regular, repetitive internal structure. The concept of symmetry describes the repetition of structural features. Symmetries are most frequently used to classify the different crystal structures. In general one can generate 14 basic crystal structures through symmetries. These are called Bravais lattices. Any crystal structures can be reduced to one of these 14 Bravias lattices.
5
6
7 Q. The crystal structure of SrTiO 3 is cubic, space group Pm3m with a unit cell edge a = 3.90 Å. Calculate the expected 2θ positions of the first three peaks in the diffraction pattern, if the radiation is Cu K α (λ = 1.54 Å). A. 1. Recognize the hkl values for the first few peaks: 100, 110, 111, 200, 210, 211, 220, etc. 2. Calculate the interplanar spacing, d, for each peak: 1/d 2 = (h 2 + k 2 + l 2 )/a 2 3. Use Bragg s Law to determine the 2θ value: λ = 2d hkl sin θ hkl hkl = 100 1/d 2 = ( )/(3.90 Å) 2 d = 3.90 Å sin θ 100 = 1.54 Å/{2(3.90 Å)} θ = 11.4 (2θ = 22.8 ) hkl = 110 1/d 2 = ( )/(3.90 Å) 2 d = 2.76 Å sinθ 110 = 1.54 Å/{2(2.76 Å)} θ = 16.2 (2θ = 32.4 ) hkl = 111 1/d 2 = ( )/(3.90 Å) 2 d = 2.25 Å sin θ 111 = 1.54 Å/{2(2.25 Å)} θ = 20.0 (2θ = 40.0 )
8
9 Powder Diffraction: Indexing Indexing is the process of determining the unit cell parameters from the peak positions. To index a powder diffraction pattern it is necessary to assign Miller indices, hkl, to each peak. A diffraction pattern cannot be analyzed until it has been indexed. It is always the first step in analysis. Unfortunately it is not just the simple reverse of calculating peak positions from the unit cell dimensions and wavelength. We will show how one can manually index diffraction patterns of high symmetry structures. For lower symmetry structures (monoclinic, triclinic) it is usually necessary to use a computer algorithm. This is called Autoindexing. The information in an XRD pattern is a direct result of two things: 1. The size and shape of the unit cells, which determine the relative positions of the diffraction peaks. 2. Atomic positions within the unit cell, which determine the relative intensities of the diffraction peaks
10
11 Bragg s Law tells us the location of a peak with indices hkl. θ hkl is related to the interplanar spacing, d, as follows: λ = 2d hkl sin θ hkl 1/d = 2 sin θ/ λ 1/d 2 = 4 sin 2 θ/λ 2 We know that for a cubic phase the dvalues can be calculated from the Miller indices (hkl): 1/d 2 = (h 2 + k 2 + l 2 )/a 2 Combining these two equations we get the following relationship or (h 2 + k 2 + l 2 ) / a 2 = 4sin 2 θ / λ 2 sin 2 θ = (λ 2 /4a 2 )(h 2 + k 2 + l 2 ) Where λ and a are constants, hence λ 2 /4a 2 is constant. Sin 2 θ is proportional to h 2 + k 2 + l 2 i.e., planes with higher Miller indices will diffract at higher values of θ.
12 In cubic systems, the first XRD peak in the diffraction pattern will be due to diffraction from planes with the lowest Miller indices simple cubic, (100), h 2 + k 2 + l 2 = 1 bodycentered cubic, (110), h 2 + k 2 + l 2 = 2 facecentered, (111), h 2 + k 2 + l 2 = 3 If the lattice is not primitive certain classes of hkl peaks will be missing. These are called systematic absences and we can use them to determine the space group (or at least narrow down the possibilities). Conditions for allowed reflection for cubic lattices: Primitive: All possible h, k and l values Bodycentered: reflection is allowed when (h + k + l) is even reflection is not allowed when (h + k + l) is odd Facecentered: reflection is allowed when h, k and l are either all even or all odd no reflection when h, k and l are mixed i.e., even and odd
13 Hence, Primitive h 2 + k 2 + l 2 = 1,2,3,4,5,6,8,9,10,11,12,13,14,16 Bodycentered h 2 + k 2 + l 2 = 2,4,6,8,10,12,14,16 Facecentered h 2 + k 2 + l 2 = 3,4,8,11,12,16,19,20,24,27,32
14 Systematic Absences Screws & Glides Screw axes and glide planes also have elements of translation and they will give systematic absences as well. Some examples are given below. Centering Allowed peaks 2 1 screw axis to a h00 peaks are only allowed when h is an even # 2 1 screw axis to b 0k0 peaks are only allowed when k is an even # 2 1 screw axis to c 00l peaks are only allowed when l is an even # 3 1 screw axis to c 00l peaks are only allowed when l = 3n (n = integer) 4 1 screw axis to c 00l peaks are only allowed when l = 4n (n = integer) a glide plane c hk0 peaks are only allowed when h is an even # b glide plane c hk0 peaks are only allowed when k is an even # n glide plane c hk0 peaks are only allowed when h+k is an even # a glide plane b h0l peaks are only allowed when h is an even # c glide plane b h0l peaks are only allowed when l is an even # n glide plane b h0l peaks are only allowed when h+l is an even #
15 Selection Rules for Reflections in Cubic Crystals (hkl) h 2 + k 2 + l 2 SC BCC FCC , , ,
16 Two Methods of Indexing 1. Mathematical 2. Analytical
17
18
19
20
21
22
23
24
25
26
27
28
29
30
31
32
33
34
35
36 Tetragonal System In this system, the sin 2 θ values obey the following relation: sin 2 θ = A (h 2 + k 2 ) + Cl 2 where A ( = λ 2 /4a 2 ) and C (= λ 2 /4c 2 ) are constants for any pattern. First of all these constants (A and C) are found which will then disclose the cell parameters a and c and enable the line indices to be calculated. The value of A is obtained from the hk0 lines. When l = 0 the above equation becomes: sin 2 θ = A (h 2 + k 2 ) The permissible values of (h 2 + k 2 ) are 1, 2, 4, 5, 8, etc. Therefore the hk0 lines must have sin 2 θ values in the ratio of these integers and A will be some number which is 1, 1/2, 1/4, 1/5, 1/8, etc., times the sin 2 θ values of these lines. C is obtained from the other lines on the pattern and by the use of the following equation. sin 2 θ A (h 2 + k 2 ) = Cl 2 Differences represented by the lefthand side of the equation are set up, for various assumed values of h and k, in an attempt to find a consistent set of Cl 2 values, which must be in the ratio of 1, 4, 9, 16, etc. Once these values are found, C can be calculated.
37 Autoindexing Manual indexing of cubic unit cells is a reasonably straightforward process. Tetragonal, trigonal and hexagonal cells can also be indexed manually with some experience, but it is not a trivial exercise. Generally indexing is done using a computer program. This process is called autoindexing. The input for an autoindexing program is typically: The peak positions (ideally lines) The wavelength The uncertainty in the peak positions The maximum allowable unit cell volume
38 Autoindexing Software A number of the most useful autoindexing programs have been gathered together by Robin Shirley into a single package called Crysfire. You can download Crysfire from the web and find tutorials on its use at To index a powder diffraction pattern try the following steps: Fit the peaks using a program such as XFit ( Take the Xfit output file and convert to a Crysfire input file, as described on the web. Run Crysfire to look for the best solutions. Evaluate the systematic absences and refine the cell parameters. This can be done using the material in the front of the international tables for crystallography or using a program like Chekcell (
39 Autoindexing  Pitfalls Inaccurate data Impurities Try different programs Drop out various weak peaks Try different sample preps Complimentary analysis Psuedosymmetry Unit cell dimensions are close to a more symmetric crystal system Inadequate number of peaks You really need peaks, particularly if the symmetry is low How do I know when I m finished? Evaluate output based on figure of merit, when the following conditions are met the solution warrants close consideration M 20 > 10 All of the peaks are indexed Solutions with figures of merit above 20 or so almost always have some degree of the truth in them, but closely related solutions and partially correct solutions are common. Favor high symmetry solutions over low symmetry ones.
40 Determination of Number of Atoms in a Unit Cell In structure determination process, the next step after establishing the shape and size of the unit cell is to find the number of atoms in the unit cell, because the number of atoms must be known before their positions can be determined. When the unit cell volume, calculated from the lattice parameters, is multiplied by the measured density of the substance it gives the weight of all the atoms in the cell. V A = ρ Where A is the sum of the atomic weights of the atoms in the unit cell, ρ is the density (g/cm 3 ) and V is the volume of the unit cell (Å 3 ). If the substance is an element of atomic weight A, then A = n 1 A Where n1 is the number of atoms per unit cell. If the substance is a chemical compound then A = n 2 M
41 Where n2 is the number of molecules per unit cell and M the molecular weight. The number of atoms per unit cell can then be calculated from n2 and the composition of the phase. Volume of the Unit Cell The following equations are used to calculate the volume V of the unit cell: Cubic: V = a 3 Tetragonal: Orthorhombic: Monoclinic: Hexagonal: V = a 2 c V = abc V = abc sinβ V = 0.866a 2 c
Reading. Chapter 12 in DeGraef and McHenry Chapter 3i in Engler and Randle
Class 17 Xray Diffraction Chapter 1 in DeGraef and McHenry Chapter 3i in Engler and Randle Reading Chapter 6 in DeGraef and McHenry (I WILL ASSUME THAT YOU KNOW ABOUT THIS CONCEPT ALREADY! IF NOT, READ
More informationXRay Diffraction HOW IT WORKS WHAT IT CAN AND WHAT IT CANNOT TELL US. Hanno zur Loye
XRay Diffraction HOW IT WORKS WHAT IT CAN AND WHAT IT CANNOT TELL US Hanno zur Loye Xrays are electromagnetic radiation of wavelength about 1 Å (1010 m), which is about the same size as an atom. The
More informationCrystals are solids in which the atoms are regularly arranged with respect to one another.
Crystalline structures. Basic concepts Crystals are solids in which the atoms are regularly arranged with respect to one another. This regularity of arrangement can be described in terms of symmetry elements.
More informationXray diffraction: theory and applications to materials science and engineering. Luca Lutterotti
Xray diffraction: theory and applications to materials science and engineering Luca Lutterotti luca.lutterotti@unitn.it Program Part 1, theory and methodologies: General principles of crystallography
More informationLMB Crystallography Course, 2013. Crystals, Symmetry and Space Groups Andrew Leslie
LMB Crystallography Course, 2013 Crystals, Symmetry and Space Groups Andrew Leslie Many of the slides were kindly provided by Erhard Hohenester (Imperial College), several other illustrations are from
More informationCHAPTER 3 THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS
CHAPTER THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS Fundamental Concepts.6 Show that the atomic packing factor for HCP is 0.74. The APF is just the total sphere volumeunit cell volume ratio.
More informationExperiment: Crystal Structure Analysis in Engineering Materials
Experiment: Crystal Structure Analysis in Engineering Materials Objective The purpose of this experiment is to introduce students to the use of Xray diffraction techniques for investigating various types
More informationChapter 2 Crystal Lattices and Reciprocal Lattices
Chapter 2 Crystal Lattices and Reciprocal Lattices Abstract In this chapter, the basic unit vectors in real space and the basic unit vectors in reciprocal space, as well as their reciprocal relationships,
More informationPOWDER XRAY DIFFRACTION: STRUCTURAL DETERMINATION OF ALKALI HALIDE SALTS
EXPERIMENT 4 POWDER XRAY DIFFRACTION: STRUCTURAL DETERMINATION OF ALKALI HALIDE SALTS I. Introduction The determination of the chemical structure of molecules is indispensable to chemists in their effort
More informationElementary Crystallography for XRay Diffraction
Introduction Crystallography originated as the science of the study of crystal forms. With the advent of the xray diffraction, the science has become primarily concerned with the study of atomic arrangements
More informationMAE 20 Winter 2011 Assignment 2 solutions
MAE 0 Winter 0 Assignment solutions. List the point coordinates of the titanium, barium, and oxygen ions for a unit cell of the perovskite crystal structure (Figure.6). In Figure.6, the barium ions are
More informationTHE STRUCTURE OF CRYSTALLINE SOLIDS. IE114 Materials Science and General Chemistry Lecture3
THE STRUCTURE OF CRYSTALLINE SOLIDS IE114 Materials Science and General Chemistry Lecture3 Outline Crystalline and Noncrystalline Materials 1) Single, Polycrystalline, Noncrystalline solids 2) Polycrystalline
More information0% (0 out of 5 correct) The questions marked with symbol have not been graded.
Page 1 of 15 0% (0 out of 5 correct) The questions marked with symbol have not been graded. Responses to questions are indicated by the symbol. 1. Which of the following materials may form crystalline
More informationCrystal Symmetries METE 327 Physical Metallurgy Copyright 2008 Loren A. Jacobson 5/16/08
Crystal Symmetries Why should we be interested? Important physical properties depend on crystal structure Conductivity Magnetic properties Stiffness Strength These properties also often depend on crystal
More informationBasic Concepts of Crystallography
Basic Concepts of Crystallography Language of Crystallography: Real Space Combination of local (point) symmetry elements, which include angular rotation, centersymmetric inversion, and reflection in mirror
More informationPowder XRay Diffraction (Powder XRD) [6.3.2]
Powder XRay Diffraction (Powder XRD) [6.3.2] Introduction to Powder XRD Powder XRay Diffraction was developed as a technique that could be applied where traditional singlecrystal diffraction cannot
More informationSolid State Theory Physics 545
Solid State Theory Physics 545 CRYSTAL STRUCTURES Describing periodic structures Terminology Basic Structures Symmetry Operations Ionic crystals often have a definite habit which gives rise to particular
More informationRelevant Reading for this Lecture... Pages 8387.
LECTURE #06 Chapter 3: Xray Diffraction and Crystal Structure Determination Learning Objectives To describe crystals in terms of the stacking of planes. How to use a dot product to solve for the angles
More informationPrecession photograph
Precession photograph Spacing of spots is used to get unit cell dimensions. Note symmetrical pattern. Crystal symmetry leads to diffraction pattern symmetry. Groups Total For proteins Laue group 230 space
More informationChapters 2 and 6 in Waseda. Lesson 8 Lattice Planes and Directions. Suggested Reading
Analytical Methods for Materials Chapters 2 and 6 in Waseda Lesson 8 Lattice Planes and Directions Suggested Reading 192 Directions and Miller Indices Draw vector and define the tail as the origin. z Determine
More informationIntroduction to Powder XRay Diffraction History Basic Principles
Introduction to Powder XRay Diffraction History Basic Principles Folie.1 History: Wilhelm Conrad Röntgen Wilhelm Conrad Röntgen discovered 1895 the Xrays. 1901 he was honoured by the Noble prize for
More informationStructure Factors 59553 78
78 Structure Factors Until now, we have only typically considered reflections arising from planes in a hypothetical lattice containing one atom in the asymmetric unit. In practice we will generally deal
More informationIntroduction to XRay Powder Diffraction Data Analysis
Introduction to XRay Powder Diffraction Data Analysis Center for Materials Science and Engineering at MIT http://prism.mit.edu/xray An Xray diffraction pattern is a plot of the intensity of Xrays scattered
More informationCrystal symmetry X nd setting X Xm m mm2 4mm 3m 6mm 2 or. 2m m2 3m m even X2 + centre Xm +centre.
III Crystal symmetry 33 Point group and space group A. Point group 1. Symbols of the 32 three dimensional point groups General Triclinic Monoclinic Tetragonal Trigonal Hexagonal Cubic symbol 1 st setting
More information12.524 2003 Lec 17: Dislocation Geometry and Fabric Production 1. Crystal Geometry
12.524 2003 Lec 17: Dislocation Geometry and Fabric Production 1. Bibliography: Crystal Geometry Assigned Reading: [Poirier, 1985]Chapter 2, 4. General References: [Kelly and Groves, 1970] Chapter 1. [Hirth
More informationCHAPTER 3: CRYSTAL STRUCTURES
CHAPTER 3: CRYSTAL STRUCTURES Crystal Structure: Basic Definitions  lecture Calculation of material density selfprep. Crystal Systems lecture + selfprep. Introduction to Crystallography lecture + selfprep.
More informationLecture 2. Surface Structure
Lecture 2 Surface Structure Quantitative Description of Surface Structure clean metal surfaces adsorbated covered and reconstructed surfaces electronic and geometrical structure References: 1) Zangwill,
More informationChapter 3. 1. 3 types of materials amorphous, crystalline, and polycrystalline. 5. Same as #3 for the ceramic and diamond crystal structures.
Chapter Highlights: Notes: 1. types of materials amorphous, crystalline, and polycrystalline.. Understand the meaning of crystallinity, which refers to a regular lattice based on a repeating unit cell..
More informationSolid State Device Fundamentals
Solid State Device Fundamentals ENS 345 Lecture Course by Alexander M. Zaitsev alexander.zaitsev@csi.cuny.edu Tel: 718 982 2812 Office 4N101b 1 Solids Three types of solids, classified according to atomic
More informationChapter 7: Basics of Xray Diffraction
Providing Solutions To Your Diffraction Needs. Chapter 7: Basics of Xray Diffraction Scintag has prepared this section for use by customers and authorized personnel. The information contained herein is
More informationChapter 3: Structure of Metals and Ceramics. Chapter 3: Structure of Metals and Ceramics. Learning Objective
Chapter 3: Structure of Metals and Ceramics Chapter 3: Structure of Metals and Ceramics Goals Define basic terms and give examples of each: Lattice Basis Atoms (Decorations or Motifs) Crystal Structure
More informationBasics in Xray Diffraction and Special Application
Basics in Xray Diffraction and Special Application Introduction: Xray Diffraction (XRD) helps one to reach the science at atomic scale in the analysis of crystal structure, chemical composition, and
More informationSpace group symmetry
Space group symmetry Screw axes Sometimes also referred to as rototranslation axes Screw axes, notation nr, involve a rotation by 360º/n about an unit cell axis followed by translation parallel to that
More informationTHE STRUCTURE OF CRYSTALLINE SOLIDS
CHAPTER 3 THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS Fundamental Concepts 3.1 What is the difference between atomic structure and crystal structure? Atomic structure relates to the number of
More informationSymmetry. From: Lipson/Cochran, The Determination of Crystal Structures
Symmetry A body is said to be symmetrical when it can be divided into parts that are related to each other in certain ways. The operation of transferring one part to the position of a symmetrically related
More informationPart 5 Space groups. 5.1 Glide planes. 5.2 Screw axes. 5.3 The 230 space groups. 5.4 Properties of space groups. 5.5 Space group and crystal structure
Part 5 Space groups 5.1 Glide planes 5.2 Screw axes 5.3 The 230 space groups 5.4 Properties of space groups 5.5 Space group and crystal structure Glide planes and screw axes 32 point groups are symmetry
More informationRetained Austenite: NonDestructive Analysis by XRD and ASTM E Dr. Alessandro Torboli  XRay Marketing Manager
Retained Austenite: NonDestructive Analysis by XRD and ASTM E97503 Dr. Alessandro Torboli  XRay Marketing Manager Outline Introduction to XRay Diffraction Retained Austenite Retained Austenite by
More informationXray Powder Diffraction Pattern Indexing for Pharmaceutical Applications
The published version of this manuscript may be found at the following webpage: http://www.pharmtech.com/pharmtech/peerreviewed+research/xraypowderdiffractionpatternindexingfor Phar/ArticleStandard/Article/detail/800851
More informationXray Diffraction (XRD)
Xray Diffraction (XRD) 1.0 What is Xray Diffraction 2.0 Basics of Crystallography 3.0 Production of Xrays 4.0 Applications of XRD 5.0 Instrumental Sources of Error 6.0 Conclusions Bragg s Law n l =2dsinq
More informationBCM 6200  Protein crystallography  I. Crystal symmetry Xray diffraction Protein crystallization Xray sources SAXS
BCM 6200  Protein crystallography  I Crystal symmetry Xray diffraction Protein crystallization Xray sources SAXS Elastic Xray Scattering From classical electrodynamics, the electric field of the electromagnetic
More informationChapter 3: The Structure of Crystalline Solids
Sapphire: cryst. Al 2 O 3 Insulin : The Structure of Crystalline Solids Crystal: a solid composed of atoms, ions, or molecules arranged in a pattern that is repeated in three dimensions A material in which
More informationCrystal Structure. A(r) = A(r + T), (1)
Crystal Structure In general, by solid we mean an equilibrium state with broken translation symmetry. That is a state for which there exist observables say, densities of particles with spatially dependent
More informationTheory of XRay Diffraction. Kingshuk Majumdar
Theory of XRay Diffraction Kingshuk Majumdar Contents Introduction to XRays Crystal Structures: Introduction to Lattices Different types of lattices Reciprocal Lattice Index Planes XRay Diffraction:
More informationXRAY DIFFRACTION PROCEDURES
XRAY DIFFRACTION PROCEDURES For Polycrystalline and Amorphous Materials HAROLD P. KLUG HEAD OF THE DEPARTMENT OF RESEARCH IN CHEMICAL PHYSICS LEROY E. ALEXANDER SENIOR FELLOW IN XRAY DIFFRACTION Mellon
More informationIntroduction to Xray Diffraction (XRD) Learning Activity
Introduction to Xray Diffraction (XRD) Learning Activity Basic Theory: Diffraction and Bragg s Law Take a look at the diagram below: Xrays Interacting with Material A Scatter Single Particle B Diffraction
More informationESS 212: Laboratory 2 and 3. For each of your paper models, assign crystallographic axes that will serve to orient the model.
ESS 212: Laboratory 2 and 3 Lab Topics: Point groups of symmetry Crystal systems and Crystallographic axes Miller Indices of crystal faces; crystal forms Exercises to be handed in: In these two labs you
More informationinterstitial positions
Interstitial Sites In the spaces between the sites of the closest packed lattices (planes), there are a number of well defined interstitial positions: The CCP (FCC) lattice in (a) has 4 octahedral, 6coordinate
More informationA crystalline solid is one which has a crystal structure in which atoms or ions are arranged in a pattern that repeats itself in three dimensions.
CHAPTER ATOMIC STRUCTURE AND BONDING. Define a crstalline solid. A crstalline solid is one which has a crstal structure in which atoms or ions are arranged in a pattern that repeats itself in three dimensions..2
More informationQuick Guide for Data Collection on the NIU Bruker Smart CCD
Quick Guide for Data Collection on the NIU Bruker Smart CCD 1. Create a new project 2. Optically align the crystal 3. Take rotation picture 4. Collect matrix to determine unit cell 5. Refine unit cell
More informationChapter Outline. How do atoms arrange themselves to form solids?
Chapter Outline How do atoms arrange themselves to form solids? Fundamental concepts and language Unit cells Crystal structures Simple cubic Facecentered cubic Bodycentered cubic Hexagonal closepacked
More informationXray thinfilm measurement techniques
Technical articles Xray thinfilm measurement techniques II. Outofplane diffraction measurements Toru Mitsunaga* 1. Introduction A thinfilm sample is twodimensionally formed on the surface of a substrate,
More informationThe University of Western Ontario Department of Physics and Astronomy P2800 Fall 2008
P2800 Fall 2008 Questions (Total  20 points): 1. Of the noble gases Ne, Ar, Kr and Xe, which should be the most chemically reactive and why? (0.5 point) Xenon should be most reactive since its outermost
More informationChem 106 Thursday Feb. 3, 2011
Chem 106 Thursday Feb. 3, 2011 Chapter 13: The Chemistry of Solids Phase Diagrams  (no BornHaber cycle) 2/3/2011 1 Approx surface area (Å 2 ) 253 258 Which C 5 H 12 alkane do you think has the highest
More informationCrystal Structure of High Temperature Superconductors. Marie Nelson East Orange Campus High School NJIT Professor: Trevor Tyson
Crystal Structure of High Temperature Superconductors Marie Nelson East Orange Campus High School NJIT Professor: Trevor Tyson Introduction History of Superconductors Superconductors are material which
More informationTwinning and absolute structure. Bill Clegg Newcastle University, UK. SHELX Workshop Denver 2016
Twinning and absolute structure Bill Clegg Newcastle University, UK SHELX Workshop Denver 2016 Outline Twinning Definition, characterisation, illustration Classification: different types of twin Recognition:
More informationBasics of Xray diffraction: From symmetry to structure determination
Basics of Xray diffraction: From symmetry to structure determination T. N. Guru Row Solid State and Structural Chemistry Unit Indian Institute of Science Bangalore560012 Email: ssctng@sscu.iisc.ernet.in
More informationData Collection and Data Reduction Techniques for Modulated Structures. Michael Ruf, Charles Campana Bruker AXS Inc., Madison, WI
Data Collection and Data Reduction Techniques for Modulated Structures Michael Ruf, Charles Campana Bruker AXS Inc., Madison, WI Dr. Michael Ruf Product Manager Single Crystal Diffraction 2 Dr. Charles
More informationSimple vs. True. Simple vs. True. Calculating Empirical and Molecular Formulas
Calculating Empirical and Molecular Formulas Formula writing is a key component for success in chemistry. How do scientists really know what the true formula for a compound might be? In this lesson we
More informationDiffraction Course Series 2015
Diffraction Course Series 2015 Mark Wainwright Analytical Centre Kensington Campus, Chemical Sciences Building F10, Room G37 The Mark Wainwright Analytical Centre is offering a new series of courses covering
More informationStructure of materials
Structure of materials The atomic number is the number of protons for each element. Atoms of the same element have the same number of protons in the nucleus but may differ by one or more neutrons forming
More informationTypes of Solids. Metallic and Ionic Solids. Crystal Lattices. Properties of Solids. Cubic Unit Cells. Metallic and Ionic Solids
1 Metallic and Ionic Solids 1 Types of Solids Table 13.6 2 TYPE EXAMPLE FORCE Ionic NaCl, CaF 2, ZnS Ionion Metallic Na, Fe Metallic Molecular Ice, I 2 Dipole Ind. dipole Network Diamond Extended Graphite
More informationXray diffraction techniques for thin films
Xray diffraction techniques for thin films Rigaku Corporation Application Laboratory Takayuki Konya 1 Today s contents (PM) Introduction Xray diffraction method OutofPlane InPlane Pole figure Reciprocal
More informationEarth Sciences: Course Presenters
Earth Sciences: Course Presenters 625102 Geology Dr Stephen Gallagher Prof Andrew Gleadow Dr Malcolm Wallace Prof Ian Plimer Course Coordinator Room 214 Series  Lecture Topics 1. Mineralogy and Crystals
More informationThe Crystal Structures of Solids
The Crystal Structures of Solids Crystals of pure substances can be analyzed using Xray diffraction methods to provide valuable information. The type and strength of intramolecular forces, density, molar
More information9/18/2013. Symmetry Operations and Space Groups. Crystal Symmetry. Symmetry Elements. Center of Symmetry: 1. Rotation Axis: n. Center of Symmetry: 1
Symmetry Operations and rystal Symmetry 32 point groups of crystals compatible with 7 crystal systems crystallographers use ermannmauguin symmetry symbols arl ermann German 89896 harlesvictor Mauguin
More informationXRay Diffraction and Crystal Structure
XRay Diffraction and Crystal Structure XRay Diffraction and Crystal Structure (XRD) Xray diffraction (XRD) is one of the most important nondestructive tools to analyse all kinds of matter  ranging
More informationEarth and Planetary Materials
Earth and Planetary Materials Spring 2013 Lecture 11 2013.02.13 Midterm exam 2/25 (Monday) Office hours: 2/18 (M) 1011am 2/20 (W) 1011am 2/21 (Th) 11am1pm No office hour 2/25 1 Point symmetry Symmetry
More informationINTRODUCTION TO XRAY DIFFRACTION
INTRODUCTION TO XRAY DIFFRACTION Lecture 4 & 5 By Dr. J. K. Baria Professor Of Physics V. P. & R. P. T. P. Science College Vidyanagar 388 120 Knowledge Keeps the mind always young TYPES OF XRAY CAMERA
More informationSymmetryoperations, point groups, space groups and crystal structure
1 Symmetryoperations, point groups, space groups and crystal structure KJ/MV 210 Helmer Fjellvåg, Department of Chemistry, University of Oslo 1994 This compendium replaces chapter 5.3 and 6 in West. Sections
More informationCHEM 10113, Quiz 7 December 7, 2011
CHEM 10113, Quiz 7 December 7, 2011 Name (please print) All equations must be balanced and show phases for full credit. Significant figures count, show charges as appropriate, and please box your answers!
More informationCrystallization and energy relations between states of matter
Crystallization and energy relations between states of matter This text is meant as background information about how undercooling happens, and how the latent heat of crystallization has to be released
More informationLAB #1 THE CRYSTALLOGRAPHY AND MILLER INDICES
LAB #1 THE CRYSTALLOGRAPHY AND MILLER INDICES THE OBJECTIVES: 1. To study simple crystal lattices using a simulation packages. THE THEORY: Solid state semiconductor technology has brought valuable systems
More informationXray Diffraction and EBSD
Xray Diffraction and EBSD Jonathan Cowen Swagelok Center for the Surface Analysis of Materials Case School of Engineering Case Western Reserve University October 27, 2014 Outline Xray Diffraction (XRD)
More informationElectron Diffraction and Crystal Structure
University of Michigan Physics 441442 2/9/06 Advanced Physics Laboratory 1. Introduction Electron Diffraction and Crystal Structure In classical mechanics we describe motion by assigning momenta to point
More informationLECTURE SUMMARY September 30th 2009
LECTURE SUMMARY September 30 th 2009 Key Lecture Topics Crystal Structures in Relation to Slip Systems Resolved Shear Stress Using a Stereographic Projection to Determine the Active Slip System Slip Planes
More informationLiquids and Solids. 1. Are liquids closer in physical properties to solids or gases? Why?
Liquids and Solids 1. Are liquids closer in physical properties to solids or gases? Why? Liquids are more similar to solids. There are many intermolecular forces experienced by solids and liquids and very
More informationEXPERIMENT 4. Microwave Experiments. Introduction. Experimental Procedure. Part 1 : Double Slit
EXPERIMENT 4 Microwave Experiments Introduction Microwaves are electromagnetic radiation in the centimeter range of wavelengths. As such, they, like light, will exhibit typical wave properties like interference
More informationNPTEL: STRUCTURE OF MATERIALS Instructor: Anandh Subramaniam [Lecture1 to Lecture45] 1. Overview (C1) (Time: 49:06)
NPTEL: STRUCTURE OF MATERIALS Instructor: Anandh Subramaniam [Lecture1 to Lecture45] Lec Chapter 1. Overview (C1) (Time: 49:06) 2. Geometry of Crystals: Symmetry, Lattices (C2) (Time: 1:08:58) 3. (Time:
More informationPart 1. XRAY DIFFRACTION MICROSTRUCTURE ANALYSIS
5 Part 1. XRAY DIFFRACTION MICROSTRUCTURE ANALYSIS 1.1. INTERACTION OF ELECTROMAGNETIC WAVES WITH MATTER The different parts of the electromagnetic spectrum have very different effects upon interaction
More informationLab 03: Precision XRay Diffractometry
Lab 03: Precision XRay Diffractometry Author: Mike Nill Alex Bryant Contents 1 Introduction 2 2 Experimental Procedures 2 3 Results 3 4 Discussion 6 4.1 Lattice Parameter Determination.............................
More informationXRay Diffraction: A Comprehensive Explanation for Multipurpose Research
XRay Diffraction: A Comprehensive Explanation for Multipurpose Research Adree Khondker 1, Shakir Lakhani 2 1 Westdale S.S., Hamilton, ON, Canada 2 Upper Canada College, Toronto, ON, Canada Abstract: The
More informationRepetitive arrangement of features (faces, corners and edges) of a crystal around
Geology 284  Mineralogy, Fall 2008 Dr. Helen Lang, West Virginia University Symmetry External Shape of Crystals reflects Internal Structure External Shape is best described by Symmetry Symmetry Repetitive
More informationPDF2 Tools and Searches
PDF2 Tools and Searches PDF2 Release 2014 The PDF2 Release 2014 database is powered by our integrated search display software. PDF2 Release 2014 boasts 55 search classifications coupled with 47 data
More informationTOPIC 8. CHEMICAL CALCULATIONS II: % composition, empirical formulas.
TOPIC 8. CHEMICAL CALCULATIONS II: % composition, empirical formulas. Percentage composition of elements in compounds. In Topic 1 it was stated that a given compound always has the same composition by
More informationXRay Diffraction. wavelength Electric field of light
Light is composed of electromagnetic radiation with an electric component that modulates versus time perpendicular to the direction it is travelling (the magnetic component is also perpendicular to the
More informationSolidstate Physics. DebyeScherrer Scan: determining the latticeplane spacings of polycrystalline powder samples. LD Physics Leaflets P7.1.2.
Solidstate Physics Properties of crystals Xray structural analysis LD Physics Leaflets P7.1..4 DebyeScherrer Scan: determining the latticeplane spacings of polycrystalline powder samples Objects of
More informationrotation,, axis of rotoinversion,, center of symmetry, and mirror planes can be
Crystal Symmetry The external shape of a crystal reflects the presence or absence of translationfree symmetry y elements in its unit cell. While not always immediately obvious, in most well formed crystal
More informationMaterials Science and Engineering Department MSE , Sample Test #1, Spring 2010
Materials Science and Engineering Department MSE 200001, Sample Test #1, Spring 2010 ID number First letter of your last name: Name: No notes, books, or information stored in calculator memories may be
More informationPSD Xray lecture 13. Overview Laue photography Xray laser femptosecond Laue photography
PSD Xray lecture 13 Overview Laue photography Xray laser femptosecond Laue photography From protein to protein structure Purify protein Grow crystals Collect Xray data Solve phase problem Refine the
More informationTOPIC 8. CHEMICAL CALCULATIONS II: % composition, empirical formulas.
TOPIC 8. CHEMICAL CALCULATIONS II: % composition, empirical formulas. Percentage composition of elements in compounds. In Topic 1 it was stated that a given compound always has the same composition by
More informationLab 31 in TFFM08. The Laue Method
IFM The Department of Physics, Chemistry and Biology Lab 31 in TFFM08 The Laue Method NAME PERS.  NUMBER DATE APPROVED Rev July 2014 ChungChuan Lai 1. Introduction Note to students: Before this lab it
More informationWe shall first regard the dense sphere packing model. 1.1. Draw a two dimensional pattern of dense packing spheres. Identify the twodimensional
Set 3: Task 1 and 2 considers many of the examples that are given in the compendium. Crystal structures derived from sphere packing models may be used to describe metals (see task 2), ionical compounds
More informationBryn Mawr College Department of Physics Undergraduate Teaching Laboratories Xray Crystallography
Bryn Mawr College Department of Physics Undergraduate Teaching Laboratories Xray Crystallography Introduction In this lab you will explore the Xray spectrum produced by copper in an Xray tube and investigate
More informationChapter 2: Crystal Structures and Symmetry
Chapter 2: Crystal Structures and Symmetry Laue, ravais December 28, 2001 Contents 1 Lattice Types and Symmetry 3 1.1 TwoDimensional Lattices................. 3 1.2 ThreeDimensional Lattices................
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationA program for phase identification using diffractograms obtained from TEM structure images
INVESTIGACIÓN Revista Mexicana de Física 59 (2013) 102 106 MARCH APRIL 2013 A program for phase identification using diffractograms obtained from TEM structure images R. Galicia a, R. Herrera a,, J. L.
More informationIntroduction to Rietveld refinements. Luca Lutterotti Department of Materials Engineering and Industrial Technologies University of Trento  Italy
Introduction to Rietveld refinements Luca Lutterotti Department of Materials Engineering and Industrial Technologies University of Trento  Italy The Rietveld method 19641966  Need to refine crystal
More informationSingle Crystal XRay Crystallography 1,2
1 Single Crystal XRay Crystallography 1,2 You will use the program APEX2 to determine the structure of an organic compound (to be referred to as Ylid) from the data supplied by our xray diffractometer.
More informationNext, solid silicon is separated from other solid impurities by treatment with hydrogen chloride at 350 C to form gaseous trichlorosilane (SiCl 3 H):
University Chemistry Quiz 5 2014/12/25 1. (5%) What is the coordination number of each sphere in (a) a simple cubic cell, (b) a bodycentered cubic cell, and (c) a facecentered cubic cell? Assume the
More informationXray diffraction. Xrays were discovered by Wilhelm Rontgen, a German physicist in 1895.
Xrays were discovered by Wilhelm Rontgen, a German physicist in 1895. To generate xrays, three things are needed. a source of electrons a means of accelerating the electrons at high speeds a target material
More information